- Nano Express
- Open Access
A promising gene delivery system developed from PEGylated MoS2 nanosheets for gene therapy
Nanoscale Research Letters volume 9, Article number: 587 (2014)
A new class of two-dimensional (2D) nanomaterial, transition metal dichalcogenides (TMDCs) such as MoS2, MoSe2, WS2, and WSe2 which have fantastic physical and chemical properties, has drawn tremendous attention in different fields recently. Herein, we for the first time take advantage of the great potential of MoS2 with well-engineered surface as a novel type of 2D nanocarriers for gene delivery and therapy of cancer. In our system, positively charged MoS2-PEG-PEI is synthesized with lipoic acid-modified polyethylene glycol (LA-PEG) and branched polyethylenimine (PEI). The amino end of positively charged nanomaterials can bind to the negatively charged small interfering RNA (siRNA). After detection of physical and chemical characteristics of the nanomaterial, cell toxicity was evaluated by 3-(4,5-dimethylthiazol-2-yl)-2,5-diphenyltetrazolium bromide (MTT) assay. Polo-like kinase 1 (PLK1) was investigated as a well-known oncogene, which was a critical regulator of cell cycle transmission at multiple levels. Through knockdown of PLK1 with siRNA carried by novel nanovector, qPCR and Western blot were used to measure the interfering efficiency; apoptosis assay was used to detect the transfection effect of PLK1. All results showed that the novel nanocarrier revealed good biocompatibility, reduced cytotoxicity, as well as high gene-carrying ability without serum interference, thus would have great potential for gene delivery and therapy.
RNA interference (RNAi) is a newly discovered cellular strategy for silencing genes in a sequence-specific manner [1–3]. At present, small interfering RNA (siRNA)-mediated gene regulation or therapy has shown immense potential in treating various diseases by silencing abnormally up-regulated genes [4–6]. In this kind of gene therapy, siRNA could be delivered into cells utilizing either viral vectors or non-viral carriers, causing degradation of targeted mRNA and subsequently leading to the silence of specific protein expression . The success of gene therapy is largely dependent on the development of a safe and efficient gene delivery system [8–10]. Viral vectors have been primarily used in gene therapy due to their high delivery efficiency [11, 12]. However, despite of the advantages such as simplicity of use, ease of large-scale production, and lack of specific immune response [13, 14], viral vectors might bring the side effects such as endogenous virus recombination, oncogenic effects, and unexpected immune response  while non-viral vectors could circumvent. Many non-viral-based gene delivery vectors, such as cationic polymers , silica nanoparticles , iron oxide nanoparticles , and many other types [19–21], have been extensively explored in recent years. Though they are widely used for research in gene delivery, their toxicity and low in vivo efficiency limited their further application .
Thus, seeking for new biological materials has become an important research direction . In recent years, nanoparticles have demonstrated unique physical and biological properties that can be applied to overcome the issues in gene and drug delivery systems due to its superior characteristics . For example, nanoparticle size is usually 10 to 100 nm, which is capable of penetrating through the submucosal layers and enhances the efficiency in gene transfection level . Besides, a number of cationic polymers have been investigated as gene carriers, such as polyethylenimine (PEI) due to its specific features. PEI has high pH-buffering capacity, lower cytotoxicity, and high transfection efficiency , thus has tremendous potential in gene therapy.
The novel nanomaterials, which could be developed from graphene or transition metal dichalcogenides (TMDCs) such as MoS2, MoSe2, WS2, and WSe2, came to be new emerging non-viral gene delivery carriers [27–30]. Graphene and its analog, TMDCs, which are the two-dimensional (2D) sp2-bonded nanocarbon with excellent electronic, optical, and mechanical properties have been extensively studied in the past decades [31, 32].
In this study, MoS2 was formulated as nanoparticles and modified by PEI on the particles to increase the surface charge, providing as a promising gene carrier candidate. The obtained positively charged MoS2-PEG-PEI could be loaded with siRNA for gene delivery. Our results for the first time suggested TMDCs as a novel type of 2D nanovector in gene delivery with low cytotoxicity and high transfection efficiency without serum interference, promising for future applications in non-viral based gene therapy.
Branched polyethylenimine (PEI) with molecular weight (MW) of 25 kDa and 3-(4,5-dimethylthiazol-2-yl)-2,5-diphenyltetrazolium bromide (MTT) were obtained from Sigma-Aldrich (St. Louis, MO, USA). Lipoic acid-modified polyethylene glycol (LA-PEG) polymers were purchased from PegBio (Suzhou, China). Lipofectamine 2000 transfection kit, 4′,6′-diamidino-2-phenylindole (DAPI), and fetal bovine serum (FBS) were obtained from Invitrogen (Carlsbad, CA, USA). Dulbecco’s modified Eagle’s medium (DMEM) was purchased from Thermo Scientific (Waltham, MA, USA). SiRNA-targeting polo-like kinase 1 (PLK1) gene and negative control siRNA with a scrambled sequence were synthesized with fluorescent label by GenePharma Co., LTD (Suzhou, China). Sequence was as follows: siPLK1, 5′-AUAUUCGA CUUUGGUUGCCdTdT-3′, siN.C., 5′-ACGUGACAC GUUCGGAGAAdTdT-3′. The entire antibodies were supplied by Abcam Co., LTD (Cambridge, MA, USA).
Synthesis of single-layer MoS2 nanosheets
MoS2 nanosheets were synthesized by the Morrison method . Shortly, 500 μg MoS2 crystal was soaked in 500 μL of 1.6 M n-butyllithium solution in hexane for 2 days inside a nitrogen glove box. Following the intercalation by lithium, the MoS2 sample was filtered and washed repeatedly with 80 mL hexane to remove excess lithium and other organic residues. Intercalated MoS2 sample was then removed immediately from glove box and ultrasonicated in water for 1 h to allow effective exfoliation, obtaining exfoliated MoS2 which was then centrifuged in 3,000 rpm to remove unexfoliated MoS2 and excess LiOH in the precipitates. The supernatant was dialyzed against deionized water using membranes with molecular weight cut-off (MWCO) of 14 kDa for 2 days to remove lithium compounds and other residue ions, obtaining MoS2 nanosheets dispersed in water for future use.
PEGylation of MoS2 nanosheets and preparation of MoS2-PEG-PEI
Ten milligrams of lipoic acid-modified PEG (LA-PEG) was added into 1 mg of MoS2 nanosheets dispersed in 2 mL of water. After sonication for 20 min and stirring overnight, excess PEG polymers were removed by centrifugal filtration with 100 kDa MWCO filters (Millipore, Billerica, MA, USA) and several times of water washing. The obtained MoS2-PEG or MoS2-PEG-FA were highly water-soluble and stored less than 4°C for use.
Generally, PEI used during this experiment was pre-dissolved in deionized water. One milligram of PEGylated MoS2 nanosheets and 0.1 mL PEI (50 mg/mL) were mixed in 2 mL deionized water. The mixture was stirred overnight under room temperature. Free PEI was removed by hyperfiltration.
Characterization of the prepared nanomaterials
Atomic force microscopy (AFM) (Veeco Inc., Plainview, NY, USA) was used to characterize the size and thickness of MoS2 nanosheets before and after PEG coating. Elemental analysis data were acquired by an elemental analyzer (EA1110 CHNO-S, Carlo Erba, Cornaredo, MI, Italy). Zeta potentials and size distributions of nanoparticles were measured by a Nano-ZS90 nanoparticle analyzer (Malvern Instruments Ltd.).
Loading of siRNA onto MoS2-PEG-PEI and agarose gel electrophoresis assay
From elemental analysis (nitrogen content), we estimated that the PEI content in MoS2-PEG-PEI conjugate was about 32%. MoS2-PEG-PEI was mixed with 20 pmol siRNA in 20 μL deionized water at different nitrogen/phosphor (N/P) ratios (N/P =0, 5, 10, 15, 20). The mixtures were then incubated for 1 h at room temperature before they were analyzed by 1% agarose gel electrophoresis in Tris-acetate-EDTA (TAE) buffer.
HepG2 cell line obtained from American Type Culture Collection (ATCC, Manassas, VA, USA) was cultured in Dulbecco’s modified Eagle’s medium (DMEM) containing 10% FBS and 1% penicillin/streptomycin at 37°C in a humidified 5% CO2-containing atmosphere.
For siRNA transfection, HepG2 cells were seeded in 35 mm culture dishes at a density of 1 × 105 cells per well. We diluted 200 pmol FAM-siRNA in 200 μL serum-containing DMEM and various concentrations of MoS2-PEG-PEI in 200-μL serum-containing DMEM. The two solutions were mixed together and incubated for 20 min at room temperature before being added into cells, maintaining the final volume at 2 mL. Here, we used Lipofectamine 2000 as the positive transfection agent and siRNA with a scrambled sequence as the negative control. After 6 h of transfection, cells were washed twice with PBS (pH = 7.4) and then imaged by a laser scanning confocal microscope (Leica SP5, Leica Microsystems, Wetzlar, Germany). The cell nuclei could be stained by DAPI. After 6 h siPLK1 without FAM label transfection following the same protocol, we transfered the cells into new fresh complete media and incubated at 37°C for additional 48 h. Cells could be stained with the calcein-AM/propidium iodide (PI) to determine the viability.
RNA extraction and quantitative real-time PCR (qPCR)
All transfected cells were washed twice with PBS and the total RNA was extracted using the TRIzol reagent (Takara, Dalian, China) according to the manufacturer’s protocol. Then, RNA was subsequently reversely transcribed to complementary DNA (cDNA) using M-MLV First-Strand cDNA Synthesis Kit (Invitrogen, Carlsbad, CA, USA). Afterwards, qPCR analysis was performed using Platinum SYBR Green qPCR SuperMix-UDG kits (Invitrogen, Carlsbad, CA, USA) on an ABI Prism 7500 Real-Time PCR system (Applied Biosystems, Foster City, CA, USA).The relative amount of PLK1 normalized to β-actin was calculated according to the 2−∆∆Ct method. Each sample was run in triplicate. The primer sequences were as follows: 5′-AGCCTGAGGCCCGATACTACCTAC-3′ (PLK1-forward), 5′-ATTAGGAGTCCCACACAGGGTCTTC-3′ (PLK1-reverse) and 5′-GCACAGAGCCTCGCCTT-3′ (β-actin-forward), 5′-GTTGTCGACGACGAGCG-3′ (β-actin -reverse).
Western blotting analysis
Total proteins were prepared by standard procedures and quantified by the Bradford BSA Protein Assay Kit. Equivalent amounts of protein were resolved and mixed with loading buffer, then loaded on 10% SDS-PAGE gel and subsequently electrotransferred to a polyvinylidene difluoride (PVDF) membrane, which was blocked for 2 h at room temperature with 5% non-fat dry milk in PBS. After blocking, the membrane was incubated with mouse anti-human PLK1 antibody at 1:1,000 at 4°C overnight followed by incubation with goat-anti-mouse IgG antibody at 1:2,000 for 1 h at room temperature. Mouse-anti-human β-actin antibody diluted at 1:1,000 was used as a control. Densitometric values of protein bands were quantified using Image Analysis software on Evolve-512 photometric system.
Flow cytometry analysis
Flow cytometry analysis was employed to quantify the cell apoptosis post treatment by using Annexin V-FITC/PI apoptosis detection kit. In details, 24 h after transfection, cells were detached by trypsin, washed with PBS, and then re-suspended in 500 μL Annexin V binding buffer containing 1 μg/L Annexin V-FITC and 4 μg/L PI. The samples were then analyzed by flow cytometry (BD FACS Calibur, BD Biosciences, San Jose, CA, USA).
Statistical analysis was performed using SPSS15.0 software. Data are expressed as the mean ± standard deviation from at least three separate experiments. Differences between groups were analyzed using Student’s t-test. A value of p <0.05 was considered statistically significant.
Results and discussion
The schematic illustration to show the construction of MoS2-PEG-PEI/siRNA is shown in Figure 1a. Two-dimensional MoS2 nanosheets were prepared by the chemical exfoliation method according to the literature . To enhance the stability of MoS2 in serum, the as-made single-layer MoS2 nanosheets were then conjugated the lipoic acid-modified PEG (LA-PEG) which is well-known for its excellent ability to prevent non-specific binding of proteins on nanomaterial surface together with the branched polyethylenimine (PEI) polymer. From elemental analysis (nitrogen content), we estimated that the PEI content in MoS2-PEG-PEI conjugate was about 32%. According to the previous studies [28, 34, 35], we used the thiol chemistry method to functionalize MoS2 nanosheets by coating the surface of MoS2 with LA-PEG which contained a disulfide group on the PEG terminal. Furthermore, the obtained positively charged MoS2-PEG-PEI could be loaded with siRNA which was negatively charged for gene delivery. To improve the physiological stability and biocompatibility of MoS2 nanosheets, surface modification of the 2D nanosheets was required before using them for bioapplications. MoS2-PEG-PEI showed excellent stability in both saline and serum-containing cell medium at room temperature (Additional file 1: Figure S1a). Consistent to this observation, MoS2-PEG-PEI kept their consistent hydrodynamic sizes at about 50 nm in the serum-containing cell medium (Additional file 1: Figure S1b). The great stability of MoS2-PEG-PEI in the presence of serum makes it a promising candidate for gene delivery without serum interference.
AFM was used to characterize MoS2 nanosheets before and after PEGylation (Figure 1b). It revealed that the original chemically-exfoliated MoS2 nanosheets showed an average diameter of ∼ 100 nm and an average thickness of ∼ 1.8 nm. After the LA-PEG coating, the average diameter of MoS2 nanosheets decreased to ∼ 50 nm because ultrasonication step might partially break down those nanosheets. However, the average thickness of PEGylated MoS2 increased to ∼ 2.8 nm, owing to the existence of PEGylation (Figure 1c). The size distributions of MoS2 before and after PEG coating are suggested by AFM images and dynamic light scattering (DLS) data in the meantime (Figures 1c and 2a).
We then evaluated the size distributions and zeta potentials of different layers of MoS2-PEG-PEI (Figure 2a,b). The zeta potentials of MoS2 and MoS2-PEG were measured to be −17.9 and −8.9 mV, respectively. MoS2-PEG-PEI with positively charged PEI coating showed an increased zeta potential of 19.9 mV. DLS data revealed that MoS2-PEG had much smaller sizes compared to original MoS2 nanosheets. And the size of MoS2-PEG-PEI was between MoS2 and MoS2-PEG.
Before we used the MoS2 nanosheets in in vitro drug delivery experiments, we tested their potential toxicity by the MTT assay which was performed to determine the relative cell viability. HepG2, HeLa, and 293 T cells were respectively incubated with various concentrations of MoS2, MoS2-PEG, and MoS2-PEG-PEI for 24 h.
In general, we found that there was no significant cytotoxicity about MoS2, PEGylated MoS2, and MoS2-PEG-PEI (Figure 3a-c). Three kinds of cells survived after 24 h incubation even under the high concentration of MoS2 up to 0.2 mg/mL. Cells which were incubated with MoS2-PEG showed higher viability compared to those which were incubated with plain MoS2. However, MoS2-PEG-PEI exhibited slightly reduced viability mainly because it was positively charged.
The above result obviously displayed that the cytotoxicity of MoS2 nanosheets, like many other nanomaterials, was closely related to their surface chemistry. Therefore, well-designed surface modification plays an important role in the biomedical application of this type of 2D nanomaterials.
Previous studies revealed that many nanoparticles could generate reactive oxygen species (ROS) such as •O2−, •OH, and H2O2 in the exposed cells, which would induce oxidative stress to harm biomolecules of cells like proteins and DNA . Thus, in order to further test the low toxicity of MoS2, PEGylated MoS2, and MoS2-PEG-PEI, intracellular ROS levels were assessed using a dihydroethidine (DHE) probe. In accord with the MTT result, no notable increase in the percentage of DHE-positive cells was observed for cells treated with MoS2, PEGylated MoS2, or MoS2-PEG-PEI for 24 h, suggesting minimal oxidative stress induced by those nanosheets (Figure 3d). Low toxicity of MoS2 nanosheets is ensured to further explore the nanomaterials as a drug carrier.
Polo-like kinase 1 (PLK1) was reported to be crucial in DNA replication [37, 38]. And it was always overexpressed in many types of cancer cells . The silencing of PLK1 would trigger cell apoptosis. Herein, we would like to use our MoS2-PEG-PEI as a nanovector for the delivery of PLK1 siRNA in order to test the transfection efficiency. To study the siRNA binding ability of our nanoparticles, we mixed MoS2-PEG-PEI with siRNA at different N/P ratios and carried out an agarose gel electrophoresis (AGE) assay (Additional file 2: Figure S2). Concluded from the AGE result, when MoS2-PEG-PEI was mixed with siRNA at N/P ratio above 5, significant retardation of siRNA movement in gel electrophoresis was observed. In contrast, bare siRNA could not be retarded.
We next used confocal fluorescence microscope to study the cellular uptake of MoS2-PEG-PEI/siRNA complex (Figure 4a). The fluorescent signal from DAPI and FAM-labeled siRNA were simultaneously detected. Clear co-localization of signals from two different channels was detected, suggesting that siRNA was successfully shuttled into cells by MoS2 nanosheets.
To determine the expression of PLK1 after MoS2-induced siRNA transfection, qPCR and Western blotting was conducted (Figure 4b,c). The qPCR result showed that lipofectamine-mediated transfection of siPLK1 (Figure 4b,c) led to a notable decrease of PLK1 compared to the control group (siN.C.). For cells treated with MoS2-PEG-PEI/siPLK1, obviously decreased PLK1 expression was observed with the increase of N/P ratio. In consistence with the qPCR result, Semi-quantification data of Western blotting (Figure 4d) uncovered that the PLK1 silencing efficiency with MoS2-PEG-PEI/siPLK1 was achieved as well as that with Lipofectamine 2000 at N/P ratio of 20, which indicated MoS2 as an effective transfection carrier.
It was documented that PLK1, as an oncogene, would trigger cell apoptosis when downregulated in cancer cells in vitro. Thus, to further ensure the onset of the MoS2 and the role of siPLK1 transfection, flow cytometry analysis was employed to quantify the cell apoptosis post treatment (Figure 5a). The results showed that an increasing proportion of apoptotic cells treated with MoS2-PEG-PEI/siPLK1 were detected with the increase of N/P ratio. Microscopy images of calcein-AM and PI double-stained (living and dead cells) HepG2 cells also showed an increasing proportion of apoptotic cells treated with MoS2-PEG-PEI/siPLK1, which had a good accordance with the flow cytometry result (Figure 5b). These results further confirmed that MoS2-PEG-PEI acted as a kind of perfect nanocarrier for gene delivery.
The success of gene therapy mostly relies on the development of the gene delivery vector . Currently, gene delivery systems are mainly categorized into viral and non-viral groups. In terms of the viral system, target genes can be packed into a virus like adenovirus, which has the capacity to inject its DNA into the host cells. However, the side effects of viral carriers, such as recombinant viral vectors reverting to their original wild type or the possibility of adverse immune responses to the host, limited their further application [42, 43]. In contrast, non-viral vectors should circumvent some of the problems occurring with the viral vectors. Moreover, non-viral vectors have advantages in simplicity of use, ease of large-scale production .
In our present study, we utilized the MoS2-based material as gene carrier. Notably, the current results exhibited TMDCs as a novel type of 2D nanovector in gene delivery with low cytotoxicity and high transfection efficiency, promising for future applications in non-viral based gene therapy. Compared with many other widely explored agents, MoS2 was an essential trace element of life. Besides, our 2D MoS2-PEG-PEI nanosheets suggest no obvious cytotoxicity. However, although preliminary in vitro experiments suggest no obvious cytotoxicity of MoS2-PEG nanosheets, we should still keep in mind that the factors controlling the pharmacokinetics and biodistribution of non-viral vectors were complicated in vivo. More deep studies were required to understand the potential toxicity as well as possible metabolism of this type of TMDC material in vivo. Thus, more attention and effort should be taken to make the perfect gene carrier suitable for clinical use.
Our work opened a novel and exciting avenue in gene delivery system. Combined with the advantages of high transfection efficiency of PEI, a new MoS2-based gene vector was successfully developed for gene therapy of cancer.
For the first time, MoS2 nanosheets with appropriate surface modification of PEG and PEI could be employed as a novel class of 2D nanocarriers for efficient siRNA delivery. And it was found that the MoS2-PEG-PEI nanosheets exhibited no observable toxicity to cells at the tested concentrations. Utilizing such a nanocarrier for PLK1 silencing, we achieved optimal gene knockdown and cancer cell apoptosis with N/P ratio of 20. Therefore, our study demonstrated that MoS2 with a well designed and engineered surface could serve as a nanocarrier that offered the novel opportunities in biomedical therapy .
Reynolds A, Leake D, Boese Q, Scaringe S, Marshall WS, Khvorova A: Rational siRNA design for RNA interference. Nat Biotech 2004, 22: 326–330. 10.1038/nbt936
Fire A, Xu S, Montgomery MK, Kostas SA, Driver SE, Mello CC: Potent and specific genetic interference by double-stranded RNA in Caenorhabditis elegans. Nature 1998, 391: 806–811. 10.1038/35888
Hannon GJ: RNA interference. Nature 2002, 418: 244–251. 10.1038/418244a
Elbashir SM, Harborth J, Lendeckel W, Yalcin A, Weber K, Tuschl T: Duplexes of 21-nucleotide RNAs mediate RNA interference in cultured mammalian cells. Nature 2001, 411: 494–498. 10.1038/35078107
Zamore PD: RNA interference: big applause for silencing in Stockholm. Cell 2006, 127: 1083–1086. 10.1016/j.cell.2006.12.001
Burnett JC, Rossi JJ: RNA-based therapeutics: current progress and future prospects. Chem Biol 2012, 19: 60–71. 10.1016/j.chembiol.2011.12.008
Felipe AV, Oliveira J, Chang PY, Moraes AA, da Silva TD, Tucci-Viegas VM, Forones NM: RNA interference: a promising therapy for gastric cancer. APJCP 2014, 15: 5509–5515.
Niidome T, Huang L: Gene therapy progress and prospects: nonviral vectors. Gene Ther 2002, 9: 1647–1652. 10.1038/sj.gt.3301923
Feng L, Yang X, Shi X, Tan X, Peng R, Wang J, Liu Z: Polyethylene glycol and polyethylenimine dual-functionalized nano-graphene oxide for photothermally enhanced gene delivery. Small 2013, 9: 1989–1997. 10.1002/smll.201202538
Vile RG, Russell SJ, Lemoine NR: Cancer gene therapy: hard lessons and new courses. Gene Ther 2000, 7: 2–8. 10.1038/sj.gt.3301084
Murlidharan G, Samulski RJ, Asokan A: Biology of adeno-associated viral vectors in the central nervous system. Front Molecular Neurosci 2014, 7: 76.
Guenther CM, Kuypers BE, Lam MT, Robinson TM, Zhao J, Suh J: Synthetic virology: engineering viruses for gene delivery. Wiley Interdiscip Rev Nanomed Nanobiotechnol 2014, 6: 548–558. 10.1002/wnan.1287
Di Pasquale E, Latronico MV, Jotti GS, Condorelli G: Lentiviral vectors and cardiovascular diseases: a genetic tool for manipulating cardiomyocyte differentiation and function. Gene Ther 2012, 19: 642–648. 10.1038/gt.2012.19
Mowa MB, Crowther C, Arbuthnot P: Therapeutic potential of adenoviral vectors for delivery of expressed RNAi activators. Expert Opin Drug Deliv 2010, 7: 1373–1385. 10.1517/17425247.2010.533655
Bessis N, GarciaCozar FJ, Boissier MC: Immune responses to gene therapy vectors: influence on vector function and effector mechanisms. Gene Ther 2004, 11(1):S10-S17.
Gao X, Huang L: Cationic liposome-mediated gene transfer. Gene Ther 1995, 2: 710–722.
Guo X, Huang L: Recent advances in nonviral vectors for gene delivery. Acc Chem Res 2011, 45: 971–979.
Arsianti M, Lim M, Marquis CP, Amal R: Assembly of polyethylenimine-based magnetic iron oxide vectors: insights into gene delivery. Langmuir 2010, 26: 7314–7326. 10.1021/la9041919
He L, Feng L, Cheng L, Liu Y, Li Z, Peng R, Li Y, Guo L, Liu Z: Multilayer dual-polymer-coated upconversion nanoparticles for multimodal imaging and serum-enhanced gene delivery. ACS Appl Mater Interfaces 2013, 5: 10381–10388. 10.1021/am403554x
Feng L, Zhang S, Liu Z: Graphene based gene transfection. Nanoscale 2011, 3: 1252–1257. 10.1039/c0nr00680g
Vankayala R, Chiang CS, Chao JI, Yuan CJ, Lin SY, Hwang KC: A general strategy to achieve ultra-high gene transfection efficiency using lipid-nanoparticle composites. Biomaterials 2014, 35: 8261–8272. 10.1016/j.biomaterials.2014.06.016
Gajbhiye V, Gong S: Lectin functionalized nanocarriers for gene delivery. Biotechnol Adv 2013, 31: 552–562. 10.1016/j.biotechadv.2013.01.005
Wang W, Li W, Ma N, Steinhoff G: Non-viral gene delivery methods. Curr Pharmaceutical Biotech 2013, 14: 46–60.
Kuo W-T, Huang H-Y, Chou M-J, Wu M-C, Huang Y-Y: Surface modification of gelatin nanoparticles with polyethylenimine as gene vector. J Nanomaterials 2011. http://dx.doi.org/10.1155/2011/646538
Desai MP, Labhasetwar V, Amidon GL, Levy RJ: Gastrointestinal uptake of biodegradable microparticles: effect of particle size. Pharmaceutical Res 1996, 13: 1838–1845. 10.1023/A:1016085108889
Goula D, Benoist C, Mantero S, Merlo G, Levi G, Demeneix BA: Polyethylenimine-based intravenous delivery of transgenes to mouse lung. Gene Ther 1998, 5: 1291–1295. 10.1038/sj.gt.3300717
Butler SZ, Hollen SM, Cao L, Cui Y, Gupta JA, Gutiérrez HR, Heinz TF, Hong SS, Huang J, Ismach AF, Johnston-Halperin E, Kuno M, Plashnitsa VV, Robinson RD, Ruoff RS, Salahuddin S, Shan J, Shi L, Spencer MG, Terrones M, Windl W, Goldberger JE: Progress, challenges, and opportunities in two-dimensional materials beyond graphene. ACS Nano 2013, 7: 2898–2926. 10.1021/nn400280c
Liu T, Wang C, Gu X, Gong H, Cheng L, Shi X, Feng L, Sun B, Liu Z: Drug delivery with PEGylated MoS2 nano-sheets for combined photothermal and chemotherapy of cancer. Adva Materials (Deerfield Beach, Fla) 2014, 26: 3433–3440. 10.1002/adma.201305256
Coleman JN, Lotya M, O’Neill A, Bergin SD, King PJ, Khan U, Young K, Gaucher A, De S, Smith RJ, Shvets IV, Arora SK, Stanton G, Kim H-Y, Lee K, Kim GT, Duesberg GS, Hallam T, Boland JJ, Wang JJ, Donegan JF, Grunlan JC, Moriarty G, Shmeliov A, Nicholls RJ, Perkins JM, Grieveson EM, Theuwissen K, McComb DW, Nellist PD, et al.: Two-dimensional nanosheets produced by liquid exfoliation of layered materials. Science 2011, 331: 568–571. 10.1126/science.1194975
Ramakrishna Matte HSS, Gomathi A, Manna AK, Late DJ, Datta R, Pati SK, Rao CNR: MoS2 and WS2 analogues of graphene. Angew Chem 2010, 122: 4153–4156. 10.1002/ange.201000009
Tang YB, Lee CS, Chen ZH, Yuan GD, Kang ZH, Luo LB, Song HS, Liu Y, He ZB, Zhang WJ, Bello I, Lee ST: High-quality graphenes via a facile quenching method for field-effect transistors. Nano Lett 2009, 9: 1374–1377. 10.1021/nl803025e
Liu X, Ma D, Tang H, Tan L, Xie Q, Zhang Y, Ma M, Yao S: Polyamidoamine dendrimer and oleic acid-functionalized graphene as biocompatible and efficient gene delivery vectors. ACS Appl Mater Interfaces 2014, 6: 8173–8183. 10.1021/am500812h
Joensen P, Frindt RF, Morrison SR: Single-layer MoS2. Mater Res Bull 1986, 21: 457–461. 10.1016/0025-5408(86)90011-5
Cheng L, Liu J, Gu X, Gong H, Shi X, Liu T, Wang C, Wang X, Liu G, Xing H, Bu W, Sun B, Liu Z: PEGylated WS2 nanosheets as a multifunctional theranostic agent for in vivo dual-modal CT/photoacoustic imaging guided photothermal therapy. Advanced Materials (Deerfield Beach, Fla) 2014, 26: 1886–1893. 10.1002/adma.201304497
Chou SS, De M, Kim J, Byun S, Dykstra C, Yu J, Huang J, Dravid VP: Ligand conjugation of chemically exfoliated MoS2. J Am Chem Soc 2013, 135: 4584–4587. 10.1021/ja310929s
Nel A, Xia T, Madler L, Li N: Toxic potential of materials at the nanolevel. Science 2006, 311: 622–627. 10.1126/science.1114397
Mandal R, Strebhardt K: PLK1: unexpected roles in DNA replication. Cell Res 2013, 23: 1251–1253. 10.1038/cr.2013.130
Mundt KE, Golsteyn RM, Lane HA, Nigg EA: On the regulation and function of human polo-like kinase 1 (PLK1): effects of overexpression on cell cycle progression. Biochem Biophys Res Commun 1997, 239: 377–385. 10.1006/bbrc.1997.7378
Pellegrino R, Calvisi DF, Ladu S, Ehemann V, Staniscia T, Evert M, Dombrowski F, Schirmacher P, Longerich T: Oncogenic and tumor suppressive roles of polo-like kinases in human hepatocellular carcinoma. Hepatology (Baltimore, Md) 2010, 51: 857–868.
Kerr JFR, Winterford CM, Harmon BV: Apoptosis. Its significance in cancer and cancer therapy. Cancer 1994, 73: 2013–2026. 10.1002/1097-0142(19940415)73:8<2013::AID-CNCR2820730802>3.0.CO;2-J
Fenske DB, MacLachlan I, Cullis PR: Long-circulating vectors for the systemic delivery of genes. Curr Opin Mol Ther 2001, 3: 153–158.
Temin HM: Safety considerations in somatic gene therapy of human disease with retrovirus vectors. Hum Gene Ther 1990, 1: 111–123. 10.1089/hum.1990.1.2-111
Sanagi T, Yabe T, Yamada H: Adenoviral gene delivery of pigment epithelium-derived factor protects striatal neurons from quinolinic acid-induced excitotoxicity. J Neuropathol Exp Neurol 2010, 69: 224–233. 10.1097/NEN.0b013e3181cfc46f
Sharma VK, Jain A, Soni V: Nano-aggregates: emerging delivery tools for tumor therapy. Crit Rev Ther Drug Carrier Syst 2013, 30: 535–563. 10.1615/CritRevTherDrugCarrierSyst.2013007706
Tao L, Long H, Zhou B, Yu SF, Lau SP, Chai Y, Fung KH, Tsang YH, Yao J, Xu D: Preparation and characterization of few-layer MoS2 nanosheets and their good nonlinear optical responses in the PMMA matrix. Nanoscale 2014, 6: 9713–9719. 10.1039/C4NR02664K
This study was supported by a grant from the National Youthful Science Foundation of China (Nos. 81302145 and 81302147) and the National Science Foundation of Jiangsu Province, China (Nos. BK20130268 and 20130270).
The authors declare that they have no competing interests.
ZK and XW generated the research idea, analyzed the data, and wrote the paper. RY and HC were involved in some of the sample preparation and material synthesis. QZ and LG performed the statistical analysis. BW and ZG provided the samples. XX, WC, and LG have given final approval of the version to be published. All authors read and approved the final manuscript.
Zhongyang Kou, Xin Wang contributed equally to this work.
Electronic supplementary material
Additional file 1: Figure S1: MoS2-PEG-PEI stability. (a) MoS2-PEG-PEI stability in water, saline, and serum-containing cell medium at room temperature. (b) MoS2-PEG-PEI kept their consistent hydrodynamic sizes at about 50 nm in the serum-containing cell medium. (TIFF 294 KB)
Additional file 2: Figure S2: Gel retardation assay. Agarose gel electrophoresis of bare siRNA, MoS2 nanosheets, and mixtures of MoS2-PEG-PEI and siRNA at different N/P ratios. Each sample was incubated at room temperature for 20 min before electrophoresis. (TIFF 112 KB)
About this article
Cite this article
Kou, Z., Wang, X., Yuan, R. et al. A promising gene delivery system developed from PEGylated MoS2 nanosheets for gene therapy. Nanoscale Res Lett 9, 587 (2014). https://doi.org/10.1186/1556-276X-9-587
- Two-dimensional (2D) nanomaterial
- MoS2 nanosheet
- RNA interference